International Journal of Engineering Inventions (IJEI)
1.
International Journal of Engineering InventionsISSN: 2278-7461, www.ijeijournal.comVolume 1, Issue 8 (October2012) PP: 31-37 AN INVESTIGATION OF NANOTUBE-INTEGRATED BUCKYSHEETS PROPERTIES WITH MOLECULAR DYNAMICS MODELING AND ANALYSIS Y. Ji1, C.J. Soong2 and Y.J. Lin1 1 Department of Mechanical Engineering, University of Texas at Tyler, Tyler, TX, USA 2 Department of Computer Science, University of Texas at Tyler, Texas, USAAbstract:––To better understand the mechanical properties of structures strengthened by carbon nanotubes integrationand/or embedding, the Young’s moduli of carbon nanotubes and carbon nanotube embedded thin structures are evaluatedusing atomic-based mechanics and molecular dynamic (MD) simulation studies in this work. Buckysheets with definedingredients with 50 mg SWNT in 500 ml surfactant-NaOH solution have been fabricated in house for the investigation withthe objectives to discovering mechanical properties alteration due to carbon nanotubes integration. The results show that theYoung’s moduli of single walled (10, 10) carbon nanotubes are ranging from 0.75 TPa to 0.9 TPa, which yields goodagreement with the relevant data in the literature. For single layer buckysheets of single-walled tubes, the simulations resultin a Young’s Modulus around 0.3 TPa. A Four-wall nanotube [(5, 5), (10, 10), (15, 15), (20, 20)] model is built to examineYoung’s modulus of multi-walled nanotubes. A slightly lower value than that of the single walled model is obtained. TheYoung’s modulus of the fabricated buckysheets exhibits similar characteristics as that of the multi-walled nanotubes’. It isalso found that the larger the separation distance between nanotubes in the buckysheet model, the smaller the value ofYoung’s modulus of the structure. The comparisons of the results between the MD simulations and the previously doneexperimental testing on buckysheets’ mechanical properties reveal some discrepancies for their Young’s moduli. The higherYoung’s moduli values for buckysheets obtained in the MD simulations are due to the exclusion of particles impurity,uneven thickness, imperfect nanotubes’ alignments, and so on. The study implies that when the fabrication techniques ofbuckysheets are continuously improved, these thin films carbon nanotube-integrated structures being created will possesshigher strengths approaching those of the nanotubes.Keywords:––Nanotubes, Buckysheets, Engineering properties, Molecular dynamics computation, Young’s moduli I. INTRODUCTION The outstanding mechanical properties of carbon nanotubes (CNTs) attracted intense researches and motivatedproposal of many applications in engineering. One of the “macroscale” forms of carbon nanotubes is the CNT thin film or“buckysheet”, has been proposed in recent years and applied in many fields, such as actuating, sensing, field emission [1],and structure damping enhancements [2]. Low density, extremely high stiffness, excellent thermal stability and large aspectratio make carbon nanotubes an ideal damping material and excellent filler candidate of composites, and we expected thatthe buckysheets have a good performance in structure damping as well. However, compared to the carbon nanotubes, themodulus of elasticity, or Young’s modulus of buckysheets was extreme small, ranging from 1.1 GPa to 24 GPa, according tosome experimental works [1], which limited the potential applications of buckysheets. In this section, we introducemolecular mechanics and dynamics simulation method to investigate the Young’s modulus (Y) of single-walled CNTs andbuckysheets. The simulation models and calculation methods were developed and/or explained, the simulation results wereanalyzed. In this paper, we apply molecular dynamics (MD) study and computer simulation techniques to help furtherunderstand the characteristic properties of carbon nanotube-fabricated, the so-called Buckysheets. Molecular Dynamics(MD) Simulation is a computer simulation technique where the time evolution of a set of interacting atoms is followed byintegrating their equations of motion, which provides a powerful tool to obtain the time-dependent properties of N-bodysystem on the nano/molecular/atomic scale [2,3]. In molecular dynamics, the classical Newtons law is used: Fi mi ai (1) dri 2here, mi is the atom mass, ai is the acceleration (ri is the position of the atom), and Fi is the force acting upon dt 2it, due to the interactions with other atoms, which is determined by the gradient of the total potential energy of the system.Given an initial set of positions and velocities, the subsequent time evolution will be completely determined. A classical algorithm for MD is the Verlet Algorithm [4]. The procedure begins by casting the system in terms of itsNewtonian equation of motion of each individual particle of the system. Verlet algorithm only considers the contribution of inter-particle potential to the force term. The inter-particle potentialis modeled as the Lennard–Jones type will be addressed in later section. The solution procedure begins with integration ofEq. (1), where a simple difference equation for the integration was employed: ri (r h) ri (t h) 2ri (t ) F (ri , j (t ))h 2 (2) i jwhere h is the time step. The particle trajectory can be readily mapped from Eq. (2) with available current and past positions.The rate-limiting step in this algorithm lies in the computation of the inter-particle force, which for a system of N particlesrequires N(N-1)/2 computations at each time step. For a given particle, many of the terms in its summation of forces will beISSN: 2278-7461 www.ijeijournal.com P a g e | 31
2.
AN INVESTIGATION OF NANOTUBE-INTEGRATED…insignificant due to a large inter-particle separation with a given potential “cutoff distance”. So, the algorithm could beaccelerated by implementing the Verlet’s neighborhood list, which selects the nearest neighbors to include in thecomputation of Eq. (2). The use of the Verlet’s neighborhood list derives a cut-off inter-particle separation, rM, beyondwhich the force terms are negligible. The criterion for the cut-off separation is given as below:r M rV nv h (3)where rv is the cut-off radius for the particle potential in units of the particle radius σ, n is chosen number of time steps, andv is a root-mean-square velocity of the particles. For a chosen n, the algorithm would proceed for n-1 time steps where onlyparticles inside a distance rM to the particle at the initial time step are included in the force term. II. MECHANICAL PROPERTIES OF NANOTUBES BY MD SIMULATIONII.1 Young’s Modulus Young’s Modulus (or elastic modulus) is one of the important mechanical properties of materials. In classicalmechanics the Young’s modulus is defined as the ratio of stress to strain before the material sample yields: F A Y (4) L L0where σ is the axial stress, ε is the strain, F is the axial tensile force acted on the objects, A is the cross-sectional area of theobject, L0 is the initial length and ΔL is the elongation under the force F.In MD simulation, we add the tensile force on the CNTs in axial direction and calculate the variation of the total potentialand length, then get the Young’s moduli of CNTs.II.2 Tensile strength Reference [5] gives a method to predict the tensile strength of single-walled carbon naotubes by MD simulation. Anano-scale finite element approach, named molecular-mechanics based finite element approach was used to derive theSWCNTs’ tensile strength as well as tensile stiffness. The nanotube strength was predicted at 77-1-1GPa with the fracturestrain around 0.3. The nanotube strength was found to be moderately dependent of the nanotube helicity, but independent ofthe nanotube diameter.II.3 Vibration propertiesThe MD simulation can give all the dynamic information (acceleration, velocity and position) of atomic system, then it hasbeen used for CNTs’ vibration properties study by many researchers [6-8]. III. STUDY BUCKYSHEET’S PROPERTIES BY MD SIMULATION The first step is to investigate the elastic and vibration properties of a cantilevered or bridged single walled carbonnanotube, as shown in Figure 1. Figure 1 (a) Cantilevered (b) and bridged single walled carbon nanotubeFor determining the natural frequencies and mode of a single-walled carbon nanotube, we consider its equivalent spaceframe-like structure under the condition of free vibration. For the problem of free vibration of an undamped structure, theequation of motion is[ M ] [ K ]y 0 y (5) where [M] and [K] are, respectively, the global mass and stiffness matrices, and {y} and are, respectively, the nodal ydisplacement vector and acceleration vector. The global stiffness matrix [K] of the frame structure can be assembled from nthe elemental stiffness matrix [K]e, i.e., [K]= [K ] e 1 e , where n is the number of beam elements. The assembling procedurefollows the node-related technique in the finite element method.ISSN: 2278-7461 www.ijeijournal.com P a g e | 32
3.
AN INVESTIGATION OF NANOTUBE-INTEGRATED… The global mass matrix [M] can be assembled from the elemental mass matrix. By considering the atomisticfeature of a carbon nanotube, the masses of electrons are neglected and the masses of carbon nuclei (mc=1.9943×10-26) areassumed to be concentrated at the centers of atoms. Then, the natural frequencies f and mode shapes are obtained from the solution of the Eigen problem([K ]s 2 [M ]s){y p } 0 (6)where, [K] s , [M] s are the condensed stiffness matrix and condensed mass matrix, respectively, {y p} is the displacementvector corresponding to the primary coordinates, i.e., the translational displacements of carbon atoms, and ω=2πf is theangular frequency. The second step, more nanotubes will be framed in a square space, they are cantilevered or bridged and entangledwith each other. The area of the square is still in nano/micro scale, with the nanotubes aspect ratio 100-1000.We are trying to simulate the mechanical properties of the nanotube system shown in Figure 2 using the same method asdescribed in the first step. Figure 2 Framed carbon nanotubes Finally, the framed “nanotube system” in Figure 2 is used as constitutive “elements” of the CNT-integrated thinfilm (or buckysheet, see the photo shot in Figure 3) and finite element method is used to model and solve the free vibrationproblem. Figure 3 Photograph of carbon nanotube-integrated thin sheet - Buckysheet (Diameter = 40mm, thickness = 30-50 microns) Multi-walled carbon nanotubes is used to fabricate buckysheets. The properties of the raw materials are listedbelow with chemical vapor deposition (CVD) technique for the synthesizing method. The material properties for thenanotubes utilized are having purity of 95%, diameter of 10~30nm, length 0.5~ 40μm, and specific surface area in the rangeof 40 – 300 m2/g. An SEM snapshot of the thin sheet fabricated is shown in Figure 4 below.ISSN: 2278-7461 www.ijeijournal.com P a g e | 33
4.
AN INVESTIGATION OF NANOTUBE-INTEGRATED… Figure 4 SEM image of a carbon nanotubes-fabricated buckysheet The SEM image of buckysheets shown above reveals that the nanotube network has composed of continuous NTropes, which is apparently the result of tube self-assembly by van der Waals force during buckysheet’s filtration process. IV. SIMULATION METHODOLOGY In the single-walled carbon nanotube model, a (10, 10) CNT was used which spanned the length of the simulationunit cell as shown in Figure 5. ε ε Figure 5 The single walled CNT simulation model and application of strains The atomic models of single and multilayer buckysheets are created using crossed geometries of single-walledcarbon nanotubes. A portion of the single layer buckysheet is shown in Figure 6. Infinitely large one is considered in thecalculations. After vacuum filtration process, the obtained CNT thin films or buckysheets consist nanotubes that are notorganized and oriented in many directions actually. Here we use an idealized atomic model which contains tube-tubeinteractions that are found in buckysheets also.ISSN: 2278-7461 www.ijeijournal.com P a g e | 34
5.
AN INVESTIGATION OF NANOTUBE-INTEGRATED… Figure 6 Atomic model of a single (crossed) layer of buckysheets For the buckysheet atomic simulation model, two (10, 10) single-walled CNTs formed a “separated cross” in a unitcell. The separation distance between the two crossed nanotubes was initially determined by minimizing the strain energy ofthe model. Under the periodic boundary conditions, the unit cell was replicated in all three dimensions.We also carried out atomic simulation of the multilayer buckysheets, where several single layer buckysheets were modeledin one unit cell and the periodic boundary conditions were applied. The separation distance among the layers was optimizedin the same way as mentioned above. The molecular mechanics/dynamics simulations calculations were performed using Cerius2/Accelrys software [9].The application of strain was performed by uniformly expanding the dimensions of the MD cell in the direction of thedeformation, then re-scaling the new coordinates of the atoms to fit within the new dimensions [10]. After the initialdeformation, the MD simulation was continued and the atoms were allowed to equilibrate within the new MD celldimensions. In the following increments of deformation, this process was repeated. In each increment, the strain energy wasminimized and recorded, then the Young’s modulus could be calculated from the second derivative of the strain energydensity with respect to various strains [11-13]: 1 E ij ( )S (7) V ijwhere V is the volume of the solid, E is the total internal energy, ij is the strain tensor, and the subscript S denotes constantentropy. V. MOLECULAR DYNAMIC SIMULATION RESULTS AND REMARKS For the single-walled CNT (10,10), the simulation results show that the Young’s modulus ranges from 0.75 TPa to0.9 TPa, which is lower than the value 0.972 TPa obtained by [10], and higher than the results (0.5~ 0.6 TPa) from [12,13].In the simulation of the single layer buckypaper, the separation distance between the crossed CNTs in the radius direction ofthe model is 3.1 nm. The Young’s Modulus of 0.3 TPa for the buckypaper was obtained. When increase the separationdistance from 2nm to 7nm between nanotubes in the buckypaper model, the value of Young’s modulus reduced from 0.349TPa to 0.267 TPa, as shown in Figure 7. 0.35 0.34 0.33 Youngs Modulus, TPa 0.32 0.31 0.3 0.29 0.28 0.27 0.26 2 2.5 3 3.5 4 4.5 5 5.5 6 6.5 7 Distance between nanotubes, A Fig. 7 Young’s modulus decreases when increase the separation distance in single layer buckysheets As to the multilayer buckysheet, the simulation results are depicted in Figure 8. The Young’s modulus decreasesfrom 0.326TPa to 0.189 TPa while the layer number of the buckysheet varies from 1 to 5, which is due to the gap betweenISSN: 2278-7461 www.ijeijournal.com P a g e | 35
6.
AN INVESTIGATION OF NANOTUBE-INTEGRATED…the buckysheets reduced the stiffness. It can be found that there is a limitation of around 0.18 Tpa in Figure 8, whichmaygive the bottom line of the buckysheets’ Young’s modulus value. 11 x 10 3.4 3.2 3 Youngs Modulus Pa 2.8 2.6 2.4 2.2 2 1.8 1 1.5 2 2.5 3 3.5 4 4.5 5 layers Fig. 8 Variation of Young’s modulus with the layer number (X axis: layers; Y axis: Young’s modulus, Tpa) The length of the carbon nanotubes was is same as that of the unit cell of the simulation model of buckysheet.Different length of single walled nantubes at 2.35, 4.8,7.25 and 9.7 nm were used to build the one-layer buckysheet modeland then the atomic simulation was accomplished to investigate its affection on the Young’s modulus of buckysheets. Wefind that the shorter the nanotubes’ length, the lower the buckysheets’ Young’s modulus, which is ranging from 0.355 TPa to0.174 TPa corresponding to the above given lengths, as shown in Figure 9. 10 x 10 3.6 3.4 3.2 3 Youngs Modulus, Pa 2.8 2.6 2.4 2.2 2 1.8 1.6 2 3 4 5 6 7 8 9 10 unit cell length,nm Fig. 9 Variation of Young’s modulus with the unit cell length (X axis: Unit cell length, nanometer; Y axis: Young’s modulus, TPa) The obtained Young’s moduli values for buckysheets were much bigger than the pervious experimental results; themost important reason for that was the simulation model disregarded lots of flaws such as impurity particles, uneventhickness and not well aligned which can significantly reduce the Young’s modulus of buckysheets; at other side, these valuemay represent the upper limit of Young’s modulus and implied that our existing fabricating method of buckysheets need tobe improved. VI. CONCLUSIONS The physical properties of carbon nanotube sheets, i.e., buckysheets were studied through finite element analysis,experimental work and atomic scale simulation, in order to find viable applications of them in structural materials, electro-mechanical systems and multifunctional systems. Buckysheets were fabricated in house using vacuum filtration techniques.SEM images showed that buckysheets created were composed of continuous nanotube ropes network, which was the resultof nanotube’s self-assembly by van der Waals force and capillary forces during filtration of the carbon nanotubes’suspension phenomena. The atomic scale and molecular dynamics simulations were employed to study the mechanicalproperties of the carbon nanotubes and buckysheets. The atomic models of carbon nanotubes and single and multilayerbuckysheets were created to investigate the molecular mechanics/dynamics of nunotubes and buckysheets so as toISSN: 2278-7461 www.ijeijournal.com P a g e | 36
7.
AN INVESTIGATION OF NANOTUBE-INTEGRATED…understand their mechanical properties. The results pointed out that for single layer buckysheets, the Young’s Modulus wasapproximately 0.3 TPa. When increasing the separation distance between nanotubes in the buckysheets model, the value ofYoung’s modulus clearly reduced. It’s found that the obtained Young’s moduli values for buckysheets were much biggerthan the experimental results we obtained previously. The most likely reason for that was that the simulation modeldisregarded lots of flaws due to impurity particles, uneven thickness and not well aligned tubes which could significantlyreduce the Young’s moduli of buckysheets. However, these higher Young’s moduli may represent potential optimumstrengths of buckysheets which motivates us to improve fabricating methods in such a way that we can take full advantagesof carbon nanotubes’ outstanding mechanical properties to benefit their integrated material strengths. REFERENCES 1. Rapaport, D.C. The art of molecular dynamics simulation, 2nd edition 2004, Cambridge University press, 2. 2004.Haile, J.M. Molecular Dynamics Simulation: Elementary Methods, 1992, John Wiley & Sons, INC. 3. Verlet, L. Computer experiments on the classical fluids. I. Thermodynamical properties of Lennard-Jones 4. Moleculars, 1967, Physical Review, 159, pp. 98-103.Sun, X. and Zhao, W. Prediction of stiffness and strength of single-walled carbon nanotubes by 5. molecular-mechanics based finite element approach, 2005, Materials Science and Engineering A, 390, pp.366- 371.Li, C. and Chou, T.-W. Single-walled carbon nanotubes as ultrahigh frequency nanomechanical resonators, 6. 2003, Physical Review B 68, 073405.Liu, P., Zhang, Y.W. and Liu, C. Oscillatory behavior of C60-nanotube oscillators: A molecular- 7. dynamics study, 2005, Journal of Applied Physics 97, 094313.Zheng, O. and Jiang, Q., Multiwalled Carbon Nanotubes as Gigahertz Oscillators, Physical Review Letters, 8. vol 88, no.4, 045503.http://www.accelrys.com/products/cerius2/ 9. Frankland, S.J.V., Harik, V.M., Odegard, G.M., Brenner, R.W. and Gates, T.S. The stress-strain10. behavior of polymer-nanotubes composites from molecular dynamics simulation, Composites Science and Technology, vol. 63, pp. 1665-1661, 2003.Lu, J.P. Elastic Properties of Carbon Nanotubes and Nanoropes, 1997, Physics Review Letters, 79, pp.1297-11. 1300.Ji, Y., Multiscale Investigations on Structural Properties and Mechanical Applications of Carbon Nanotubes12. Sheets”, 2007, Ph.D. Dissertation, University of Akron, USA.Huntington, J.B., Solid State Physics, edited by F. Seitz and D. Turnbull, 1958, 7, Academic, New York.13. Byron Pipesa P., Franklandb, S.J.V., Hubertc P. and ErikSaether, 2003, Self-consistent properties of carbon nanotubes and hexagonal arrays as composite reinforcements, 2003, Composites Science and Technology, 63, pp. 1349-1358.ISSN: 2278-7461 www.ijeijournal.com P a g e | 37
Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.
Be the first to comment